Programmable nanoengineering templates for fabrication of three-dimensional nanophotonic structures
© Lin et al.; licensee Springer. 2013
Received: 14 May 2013
Accepted: 28 May 2013
Published: 7 June 2013
Porous anodic alumina membranes (AAMs) have attracted great amount of attention due to their potential application as templates for nanoengineering. Template-guided fabrication and assembly of nanomaterials based on AAMs are cost-effective and scalable methods to program and engineer the shape and morphology of nanostructures and nanomaterials. In this work, perfectly ordered AAMs with the record large pitch up to 3 μm have been fabricated by properly controlling the anodization conditions and utilization of nanoimprint technique. Due to the capability of programmable structural design and fabrication, a variety of nanostructures, including nanopillar arrays, nanotower arrays, and nanocone arrays, have been successfully fabricated using nanoengineered AAM templates. Particularly, amorphous Si nanocones have been fabricated as three-dimensional nanophotonic structures with the characterization of their intriguing optical anti-reflection property. These results directly indicate the potential application of the reported approach for photonics and optoelectronics.
The capability to program and engineer the shape and morphology of nanostructures and nanomaterials enables tailoring their electronic[1–3], optical[4–6], sensing[7, 8], thermal[9, 10], and mechanical[11–14] properties for a variety of applications including electronics, photovoltaics, sensors, thermoelectrics, nanomechanical devices, etc. Specifically, a variety of three-dimensional (3-D) nanophotonic structures, such as nanowires[15, 16], nanopillars[17, 18], nanowells, and so forth, have been extensively studied for efficient light harvesting scheme to enhance the performance of solar cells. Properly engineered 3-D nanostructures have demonstrated highly promising capability of harvesting sunlight over a broad range of wavelengths and incident angles due to their broadband anti-reflection and efficient light trapping properties. On the other hand, cost-effective approaches toward the precise control of the shape and morphology of nanostructures are crucial for any aforementioned practical applications. In general, nanofabrication methods used to produce nanostructures are commonly defined as ‘top-down’ and ‘bottom-up’ methods. The top-down approaches, which use various kinds of lithographic techniques to pattern nanoscale structures typically in two dimensions, allow to fabricate different and complex structures with high precision. However, their major disadvantage rests in high cost and limited scalability. Conversely, the bottom-up approaches, which utilize energetic favorable self-assembly and/or self-organizing mechanisms to form nanostructures, are cost-effective but usually lack of controllability over as-obtained macro- and nanostructures. In this regard, a cost-effective and scalable method combining the advantages of both top-down and bottom-up approaches will be highly appealing. Template-guided fabrication and assembly of nanomaterials, particularly based on porous anodic alumina membranes (AAMs), have attracted great amount of attention due to the fact that AAMs are formed by self-organizing mechanism and they enable direct assembly of nanomaterials with controlled density[21–25]. Meanwhile, recent achievements on controlling template regularity and internal structure clearly demonstrate their potency for the precise integration of nanomaterials with high degree of freedom[17, 26–28]. In this work, we present the fabrication of AAMs with perfect regularity and unprecedented large pitch up to 3 μm by applying high-voltage anodization in conjunction with nanoimprint process. More importantly, due to the capability of programmable structural design and fabrication, a variety of nanostructures, including nanopillar arrays, nanotower arrays, and nanocone arrays, have been successfully fabricated using nanoengineered AAM templates. Particularly, the nanocone arrays have been demonstrated as excellent 3-D nanophotonic structures for efficient light harvesting due to the gradually changed effective refractive index.
Aluminum foil (0.25 mm thick, 99.99% purity) was obtained from Alfa Aesar (Ward Hill, MA, USA), polyimide solution (PI 2525) was purchased from HD MicroSystems (Parlin, NJ, USA), polycarbonate film (0.2 mm thick) was obtained from Suzhou Zhuonier Optical Materials Co., Ltd. (Suzhou, China), epoxy glue (Norland Optical Adhesive 81) was purchased from Norland Products Inc. (Cranbury, NJ, USA), silicone elastomer and the curing agent were purchased from Dow Corning (Midland, MI, USA). All other chemicals are products of Sigma-Aldrich (St. Louis, MO, USA).
Anodization conditions of perfectly ordered large pitch porous AAMs
230 mL, 1:1, 4 wt.% citric acid/ethylene glycol (EG) + 15 mL 0.1% H3PO4
240 mL, 1:1, 1 wt.% citric acid/EG + 1.5 mL 0.1% H3PO4
240 mL, 1:1, 0.1 wt.% citric acid/EG
240 mL, 1:1, 0.05 wt.% citric acid/EG
240 mL, 1:1, 0.05 wt.% citric acid/EG
PI nanopillar array assembly
Six hundred microliters of PI solution was dispensed on an AAM substrate. After tilting and rotating the substrate to spread the solution to achieve full substrate coverage, the substrate was spin-coated on a spin-coater (Model WS-400BZ-6NPP/LITE, Laurell Technologies Corporation, North Wales, PA, USA) at 500 rpm for 30 s first, then quickly accelerated (2,000 rpm/s) to 1,000 rpm for 30 s. After spin-coating, the substrate was transferred to a hot plate to cure PI solution, started from room temperature to 300°C with a ramping rate of 20°C/min, and maintained at 300°C for 10 min. The cured substrate was then bonded to a PC film with epoxy glue, then cured by a 4-W UV lamp (Model UVL-21 Compact UV lamp, UVP, LLC, Upland, CA, USA) for 10 h. In the end, PI nanopillar arrays were transferred to the PC film by directly peeling off the PC film from the AAM substrate.
Bonding of the a-Si nanocones device on glass and PDMS
The AAM substrate with amorphous silicon (a-Si) nanocone array deposition was attached to a glass slide with epoxy glue, then cured by a 4-W UV lamp for 10 h. The Al substrate was etched from the back side in a saturated HgCl2 solution, followed by removal of AAM in HF solution (0.5 wt.% in deionized water) with high selectivity over a-Si nanocone array. For the mechanically flexible device, instead of glass, polydimethylsiloxane (PDMS) was used for the encapsulation. To encapsulate the device with PDMS, silicone elastomer was mixed with the curing agent (10:1 weight ratio) at room temperature, then poured onto the device in a plastic dish to form an approximately 2-mm layer, and cured at 60°C for 6 h. The Al substrate and AAM were then removed sequentially by the aforementioned etching process. Finally, approximately 2-mm-thick PDMS was cured on the back side of the substrate to finish the encapsulation process.
Microscopy and spectroscopy
Scanning electron microscopy (SEM) images of uncoated or Au-coated samples were obtained using a JEOL JSM-6700 F SEM (JEOL Ltd., Akishima-shi, Japan) working at 5 kV. Ultraviolet–visible (UV–vis) spectra of all samples were recorded on a Perkin Elmer Lambda 20 UV/Vis Spectrometer (Perkin Elmer, Waltham, MA, USA). Finite-difference time-domain (FDTD) simulation was employed to confirm the reflection property of the nanocone arrays as fabricated in the experiments.
Results and discussion
Electrochemical anodization of aluminum (Al) in acidic solution to form porous alumina has been well documented[29–31]. The self-organizing mechanism typically yields nanopore arrays with a few micrometers short range hexagonal ordering[32–34]. As the process is facile and low cost, it has been widely used for assembly of nanowires and nanotubes previously[17, 21, 25–27]. Meanwhile, Masuda et al. has reported fabrication of long-range perfect-ordered AAM with pitch less than 500 nm by texturing Al surface. On the other hand, in order to fabricate nanostructures with a wide range of geometries, much larger pitch is required for a number of applications. For example, it has been shown that when photon wavelength is comparable to pitch, it can be efficiently absorbed by the three-dimensional nanowell structure. Therefore, a wide range of pitch enables efficient light-structure interaction for a broad range of wavelength. Nevertheless, perfectly ordered AAM with pitch larger than 500 nm has rarely been reported. The realization of larger pitch was rather challenging due to the ‘breakdown’ or ‘burning’ of the oxide film caused by the catastrophic flow of electric current under higher anodization voltages[36, 37]. Recently, we have reported perfectly ordered AAM with pitch up to 2 μm for efficient photon harvesting[19, 28]. In this work, we have extended the largest pitch up to 3 μm. The detailed fabrication procedure of hexagonally ordered porous AAM is schematically shown in Figure 1a. Briefly, an Al sheet was polished electrochemically before being imprinted using a Si mold with a hexagonally arranged array of nanopillars, followed by the first anodization with stable high voltage to get ordered anodic alumina channels. The first anodization layer was then etched away (first etch) followed by the second anodization under the same conditions; in this case, the imprinted texture on the top can be removed, leaving the naturally developed porous structure with cone-shape opening. The diameter of the nanopores on the second anodization layer can be controllably widened to desirable size, as shown in Additional file1: Figure S1a,b. Note that since pitches of structures are larger than 1 μm, the Si imprint molds are fabricated with wafer stepper instead of electron beam lithography, thus the molds can be made into large size with high throughput. Figure 1b demonstrates the top-view SEM image of Al concave structure after the removal of the first anodization layer, clearly showing the hexagonal periodicity caused by nanoimprint has been transferred to Al below the first anodization layer of AAM. Figure 1c illustrates the top-view SEM image of perfectly ordered AAM after the second anodization with cone-shape opening, which is easier to be observed from the cross-sectional view, as shown in the inset of Figure 1c.
According to the rationale discussed above, 2.5- and 3-μm-pitch AAMs were also fabricated after hundreds of trials with various anodization conditions. The best anodization conditions of these perfectly ordered large-pitch porous AAMs were summarized in Table 1. Note that as the acids are highly diluted, anodization process occurs in a quite slow rate; therefore, AAM growth rate is very slow as well, as shown in Additional file1: Figure S1d. Figure 2b,c show SEM images of ordered 2.5- and 3-μm-pitch AAM after the first anodization, instead of after the second anodization. The matching anodization potential for 3-μm-pitch AAM is 1,200 V, which generates massive heat so that the present cooling system was not powerful enough to maintain the temperature stability leading to the burning of oxide films during the anodization process gradually. Therefore, the maximum depth of the channels in 3-μm-pitch AAM after the first anodization we achieved was about 1 μm (inset in Figure 2c). This depth is not sufficient to form deep Al concave texture to guide the self-assembly of porous alumina during the second anodization. Whereas the maximum pitch of ordered porous AAM achieved in this work is up to 3 μm, it is believed that the pitch can be further increased in the future by modifying the anodization conditions more carefully assisted with a more effective cooling system.
As the internal structure and shape of AAM nanochannels can be programmed and engineered[17, 36], it opens up more degree of freedom on AAM geometry control. In this work, AAMs with three segments with different channel diameters are fabricated by controlling etching and anodization time. Additional file1: Figure S4 illustrates the schematic process. In brief, a substrate has undergone the second anodization for time tA1 and etched for tE1 to broaden the pores and form the large-diameter segment of the membrane. Then, the third anodization step was performed for another time tA2 followed by chemical etch for time tE2 to form the medium-diameter segment. In the end, the fourth anodization step was carried out for time tA3 ending with time tE3 wet etching to form the small-diameter segment. Note that in this scenario the first segment (Figure 3d) was etched for time tE1 + tE2 + tE3, and the third segment was etched only for tE3 to broaden the pore size. In a generalized case, if there are n segments in total, the total etching time for the m th segment will be. Therefore, the diameter of the m th segment can be determined by the etching calibration curve and the fitted function (Additional file1: Figure S1a,b). In addition, the total depth of the AAM substrate is with the m th segment's depth of H m = G(tAm) which can be determined by the plots shown in Additional file1: Figure S1c,d. Figure 3d demonstrates the cross section of a 1-μm-pitch tri-diameter AAM fabricated by a four-step anodization process. Such a structure has been used to template PC nanotowers, as shown in Figure 3e,f, by the aforementioned thermal press process (Additional file1: Figure S2b). Note that as the length of each diameter segment is controllable, a smooth internal slope on the side wall can be achieved by properly shortening each segment. Therefore, a nanocone structure can be obtained, as shown in Figure 3f.
It is noteworthy that the nanocone structure is a highly promising structure for efficient light harvesting, due to the gradually changed effective refractive index, thus it has been used for improving performance of solar cells[40–42]. In this work, optical reflectance of a-Si nanocones was characterized and shown in Figure 4b. As shown in the inset of Figure 4b, 1-μm-pitch a-Si cone array on a transparent glass substrate shows black color with very low reflectance, as a comparison, a-Si thin film on the glass substrate deposited at the same time with PECVD appears to be mirror-like specular reflective. To further characterize optical properties of the a-Si nanocone array, its optical reflectance was measured with UV–vis spectroscopy equipped with an integrating sphere, together with the a-Si thin film deposited on glass for comparison. As shown in Figure 4b, the a-Si thin film on planar glass demonstrates 25 to 65% high reflectance with wavelength below 720 nm corresponding to a-Si band-gap. In contrast, the a-Si cone array has below 10% reflectance within the same wavelength range, with the minimum reflectance less than 1% at 500-nm wavelength, corresponding to peak of solar irradiance spectrum. In order to corroborate the experimental results, as well as to gain insight into the light propagation in the structures, FDTD simulations were performed on these two structures at 500-nm wavelength, with the cross-sectional electric field intensity (|E|) distribution of the electromagnetic (EM) wave plotted in Figure 4c. In the simulations, EM plane waves propagate downward from Y = 1.5 μm. Note that the color index at the specific location in the simulations reflects the magnitude of |E| at that point, normalized with that of the source EM wave if propagating in free space. It can be observed that a-Si nanocone array demonstrates quite low reflectance, indicated by the small magnitude of |E| above Y = 1.5 μm (Figure 4c). On the contrary, a-Si planar structure shows much higher reflectance (Figure 4d). Low reflectance of a-Si nanocone array indicates an efficient light absorption in the structure, which is attributed to the gradual change of its effective refractive index. In addition, as the supporting substrate can be arbitrary, flexible PDMS substrates were used and demonstrated in Figure 4e, with the schematic device structure shown in Figure 4f. This result clearly shows the promising potency of the fabricated large-pitch AAM as three-dimensional flexible template for efficient photovoltaics.
In summary, we have demonstrated fabrication of perfectly ordered AAM with the record large pitch up to 3 μm by properly controlling the anodization conditions and utilization of nanoimprint technique. By the precise structure design and control, a number of unique nanostructures, including nanopillars, nanotowers, and nanocones, have been successfully fabricated using large-pitch AAMs as nanoengineering templates. This approach can be extended to a variety of other complex structures compatible with diverse materials. Particularly, a-Si nanocones have been fabricated as 3-D nanophotonic structures with characterization of their intriguing optical anti-reflection property. These results directly indicate the potential application of the reported approach for photonics and optoelectronics.
This work was partially supported by ITS/192/11 from Hong Kong Innovation Technology Commission, HKUST Research Project Competition Grant (RPC11EG38), General Research Fund (612111) from Hong Kong Research Grant Council, and National Research Foundation of Korea funded by the Korean Government (NRF-2010-220-D00060, 2008–0662256). Supporting information is available online from Wiley InterScience or from the author.
- Hong WK, Sohn JI, Hwang DK, Kwon SS, Jo G, Song S, Kim SM, Ko HJ, Park SJ, Welland ME: Tunable electronic transport characteristics of surface-architecture-controlled ZnO nanowire field effect transistors. Nano Lett 2008, 8: 950–956. 10.1021/nl0731116View ArticleGoogle Scholar
- Chang PC, Fan ZY, Wang DW, Tseng WY, Chiou WA, Hong J, Lu JG: ZnO nanowires synthesized by vapor trapping CVD method. Chem Mater 2004, 16: 5133–5137. 10.1021/cm049182cView ArticleGoogle Scholar
- Kapadia R, Fan Z, Javey A: Design constraints and guidelines for CdS/CdTe nanopillar based photovoltaics. Appl Phys Lett 2010, 96: 103116. 10.1063/1.3340938View ArticleGoogle Scholar
- Yeh LK, Lai KY, Lin GJ, Fu PH, Chang HC, Lin CA, He JH: Giant efficiency enhancement of GaAs solar cells with graded antireflection layers based on syringelike ZnO nanorod arrays. Adv Energy Mater 2011, 1: 506–510. 10.1002/aenm.201100025View ArticleGoogle Scholar
- Chueh YL, Fan ZY, Takei K, Ko H, Kapdia R, Rathore A, Miller N, Yu K, Wu M, Haller EE, Javey A: Black Ge based on crystalline/amorphous core/shell nanoneedle arrays. Nano Lett 2010, 10: 520–523. 10.1021/nl903366zView ArticleGoogle Scholar
- Hua B, Lin Q, Zhang Q, Fan Z: Efficient photon management with nanostructures for photovoltaics. Nanoscale 2013. 10.1039/C3NR01152FGoogle Scholar
- Park W, Jo G, Hong WK, Yoon J, Choe M, Lee S, Ji Y, Kim G, Kahng YH, Lee K: Enhancement in the photodetection of ZnO nanowires by introducing surface-roughness-induced traps. Nanotechnology 2011, 22: 205204–205209. 10.1088/0957-4484/22/20/205204View ArticleGoogle Scholar
- Shaalan N, Yamazaki T, Kikuta T: Influence of morphology and structure geometry on NO2 gas-sensing characteristics of SnO2 nanostructures synthesized via a thermal evaporation method. Sensors Actuators B: Chem 2011, 153: 11–16. 10.1016/j.snb.2010.09.070View ArticleGoogle Scholar
- Hochbaum AI, Chen RK, Delgado RD, Liang WJ, Garnett EC, Najarian M, Majumdar A, Yang PD: Enhanced thermoelectric performance of rough silicon nanowires. Nature 2008, 451: 163–168. 10.1038/nature06381View ArticleGoogle Scholar
- Pichanusakorn P, Bandaru P: Nanostructured thermoelectrics. Mater Sci Eng R 2010, 67: 19–63. 10.1016/j.mser.2009.10.001View ArticleGoogle Scholar
- Stan G, Ciobanu C, Parthangal P, Cook R: Diameter-dependent radial and tangential elastic moduli of ZnO nanowires. Nano Lett 2007, 7: 3691–3697. 10.1021/nl071986eView ArticleGoogle Scholar
- Bai X, Gao P, Wang ZL, Wang E: Dual-mode mechanical resonance of individual ZnO nanobelts. Appl Phys Lett 2003, 82: 4806–4808. 10.1063/1.1587878View ArticleGoogle Scholar
- Ko H, Zhang ZX, Chueh YL, Ho JC, Lee J, Fearing RS, Javey A: Wet and dry adhesion properties of self-selective nanowire connectors. Adv Energy Mater 2009, 19: 3098–3102.Google Scholar
- Ko H, Zhang Z, Takei K, Javey A: Hierarchical polymer micropillar arrays decorated with ZnO nanowires. Nanotechnology 2010, 21: 295305–295309. 10.1088/0957-4484/21/29/295305View ArticleGoogle Scholar
- Chao Y, Chen C, Lin C, He J: Light scattering by nanostructured anti-reflection coatings. Energ Environ Sci 2011, 4: 3436–3441. 10.1039/c0ee00636jView ArticleGoogle Scholar
- Chang H, Lai K, Dai Y, Wang H, Lin C, He J: Nanowire arrays with controlled structure profiles for maximizing optical collection efficiency. Energ Environ Sci 2011, 4: 2863–2869. 10.1039/c0ee00595aView ArticleGoogle Scholar
- Fan ZY, Kapadia R, Leu PW, Zhang XB, Chueh YL, Takei K, Yu K, Jamshidi A, Rathore AA, Ruebusch DJ, Wu M, Javey A: Ordered arrays of dual-diameter nanopillars for maximized optical absorption. Nano Lett 2010, 10: 3823–3827. 10.1021/nl1010788View ArticleGoogle Scholar
- Hua B, Wang B, Leu PW, Fan ZY: Rational geometrical design of multi-diameter nanopillars for efficient light harvesting. Nano Energy 2013. 10.1016/j.nanoen.2013.03.016Google Scholar
- Leung SF, Yu M, Lin Q, Kwon K, Ching KL, Gu L, Yu K, Fan Z: Efficient photon capturing with ordered three-dimensional nanowell arrays. Nano Lett 2012, 12: 3682–3689. 10.1021/nl3014567View ArticleGoogle Scholar
- Gates BD, Xu Q, Stewart M, Ryan D, Willson CG, Whitesides GM: New approaches to nanofabrication: molding, printing, and other techniques. Chem Rev 2005, 105: 1171–1196. 10.1021/cr030076oView ArticleGoogle Scholar
- Fan ZY, Dutta D, Chien CJ, Chen HY, Brown EC, Chang PC, Lu JG: Electrical and photoconductive properties of vertical ZnO nanowires in high density arrays. Appl Phys Lett 2006, 89: 213110–213112. 10.1063/1.2387868View ArticleGoogle Scholar
- Masuda H, Fukuda K: Ordered metal nanohole arrays made by a two-step replication of honeycomb structures of anodic alumina. Science 1995, 268: 1466–1468. 10.1126/science.268.5216.1466View ArticleGoogle Scholar
- Yanagishita T, Sasaki M, Nishio K, Masuda H: Carbon nanotubes with a triangular cross-section, fabricated using anodic porous alumina as the template. Adv Mater 2004, 16: 429–432. 10.1002/adma.200306012View ArticleGoogle Scholar
- Banerjee P, Perez I, Henn-Lecordier L, Lee SB, Rubloff GW: Nanotubular metal-insulator-metal capacitor arrays for energy storage. Nat Nanotechnol 2009, 4: 292–296. 10.1038/nnano.2009.37View ArticleGoogle Scholar
- Steinhart M, Wendorff JH, Greiner A, Wehrspohn RB, Nielsch K, Schilling J, Choi J, Gosele U: Polymer nanotubes by wetting of ordered porous templates. Science 2002, 296: 1997–1997. 10.1126/science.1071210View ArticleGoogle Scholar
- Fan ZY, Razavi H, Do JW, Moriwaki A, Ergen O, Chueh YL, Leu PW, Ho JC, Takahashi T, Reichertz LA, Neale S, Yu K, Wu M, Ager JW, Javey A: Three dimensional nanopillar array photovoltaics on low cost and flexible substrate. Nat Mater 2009, 8: 648–653. 10.1038/nmat2493View ArticleGoogle Scholar
- Ergen O, Ruebusch DJ, Fang H, Rathore AA, Kapadia R, Fan Z, Takei K, Jamshidi A, Wu M, Javey A: Shape-controlled synthesis of single-crystalline nanopillar arrays by template-assisted vapor–liquid-solid process. J Am Chem Soc 2010, 132: 13972–13974. 10.1021/ja1052413View ArticleGoogle Scholar
- Lin Q, Hua B, Leung S, Duan X, Fan Z: Efficient light absorption with integrated nanopillar/nanowell arrays for three-dimensional thin-film photovoltaic applications. ACS Nano 2013, 7: 2725–2732. 10.1021/nn400160nView ArticleGoogle Scholar
- Keller F, Hunter M, Robinson D: Structural features of oxide coatings on aluminum. J Electrochem Soc 1953, 100: 411–419. 10.1149/1.2781142View ArticleGoogle Scholar
- Ebihara K, Takahashi H, Nagayama M: Structure and density of anodic oxide films formed on aluminium in oxalic acid solutions. J Met Finish Soc Jpn 1983, 34: 548–553. 10.4139/sfj1950.34.548View ArticleGoogle Scholar
- O'sullivan J, Wood G: The morphology and mechanism of formation of porous anodic films on aluminium. Proc R Soc London Ser A 1970, 317: 511–543. 10.1098/rspa.1970.0129View ArticleGoogle Scholar
- Masuda H, Yada K, Osaka A: Self-ordering of cell configuration of anodic porous alumina with large-size pores in phosphoric acid solution. Jpn J Appl Phys 1998, 37: L1340-L1342. 10.1143/JJAP.37.L1340View ArticleGoogle Scholar
- Jessensky O, Muller F, Gosele U: Self-organized formation of hexagonal pore arrays in anodic alumina. Appl Phys Lett 1998, 72: 1173–1175. 10.1063/1.121004View ArticleGoogle Scholar
- Nielsch K, Choi J, Schwirn K, Wehrspohn RB, Gösele U: Self-ordering regimes of porous alumina: the 10% porosity rule. Nano Lett 2002, 2: 677–680. 10.1021/nl025537kView ArticleGoogle Scholar
- Masuda H, Yamada H, Satoh M, Asoh H, Nakao M, Tamamura T: Highly ordered nanochannel-array architecture in anodic alumina. Appl Phys Lett 1997, 71: 2770–2772. 10.1063/1.120128View ArticleGoogle Scholar
- Lee W, Ji R, Gösele U, Nielsch K: Fast fabrication of long-range ordered porous alumina membranes by hard anodization. Nat Mater 2006, 5: 741–747. 10.1038/nmat1717View ArticleGoogle Scholar
- Ono S, Saito M, Ishiguro M, Asoh H: Controlling factor of self-ordering of anodic porous alumina. J Electrochem Soc 2004, 151: B473-B478. 10.1149/1.1767838View ArticleGoogle Scholar
- Chu S, Wada K, Inoue S, Isogai M, Katsuta Y, Yasumori A: Large-scale fabrication of ordered nanoporous alumina films with arbitrary pore intervals by critical-potential anodization. J Electrochem Soc 2006, 153: B384-B391. 10.1149/1.2218822View ArticleGoogle Scholar
- Yu R, Ching K, Lin Q, Leung S, Arcrossito D, Fan Z: Strong light absorption of self-organized 3-D nanospike arrays for photovoltaic applications. ACS Nano 2011, 5: 9291–9298. 10.1021/nn203844zView ArticleGoogle Scholar
- Garnett EC, Brongersma ML, Cui Y, McGehee MD: Nanowire solar cells. Annu Rev Mater Res 2011, 41: 269–295. 10.1146/annurev-matsci-062910-100434View ArticleGoogle Scholar
- Hsu CM, Battaglia C, Pahud C, Ruan Z, Haug FJ, Fan S, Ballif C, Cui Y: High-efficiency amorphous silicon solar cell on a periodic nanocone back reflector. Adv Energy Mater 2012, 2: 628–633. 10.1002/aenm.201100514View ArticleGoogle Scholar
- Jeong S, Garnett EC, Wang S, Yu Z, Fan S, Brongersma ML, McGehee MD, Cui Y: Hybrid silicon nanocone-polymer solar cells. Nano Lett 2012, 12: 2971–2976. 10.1021/nl300713xView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.